Size Effects In the Crushing of Honeycomb Structures


 Lambert Henry
 10 months ago
 Views:
Transcription
1 45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference April 2004, Palm Springs, California AIAA Size Effects In the Crushing of Honeycomb Structures Erik C. Mellquist * and Anthony M. Waas Composite Structures Laboratory, Aerospace Engineering Department, The University of Michigan, Ann Arbor, MI, The effect of cell size on the out of plane compressive crushing response of circular cell polycarbonate honeycomb is presented. The results are a continuation of a study originally done by Mellquist and Waas, Experiments were conducted on hexagonal cell honeycombs ranging in size from 1 to 14 cells. The results show that no scaling factor can be determined for the crushing load based on sample size, but that stability appears to be a driving property. Specimen crosssection shapes that have an arrangement of cells with higher orders of symmetry provide greater stability and are less imperfection sensitive and therefore have higher crushing loads. Finite element analysis (FEA) was used to better understand the behavior of the honeycombs during crushing and to validate experimental results. An FEA model developed during the previous work (a 7 cell model) has been expanded to multiple sizes. The results are presented and show that the model can accurately predict how different size honeycombs will perform under crushing loads. Nomenclature E = Young s modulus N = number of circular cells in a honeycomb sample n = Poisson s ratio S max = the maximum crushing stress of a honeycomb sample S plateau = the plateau crushing stress of a honeycomb sample S I. Introduction andwich structures (that employ a honeycomb core between two relatively thin skins) are desirable in several engineering applications that require high strength to weight ratios. Because of their ability to absorb large amounts of energy, they are also often used as a cushion against external loads. Honeycomb sandwich structures are currently being used in many engineering applications, both within and outside of aerospace engineering. Most studies in the literature are related to one of the attributes (high strength/weight or increased energy absorption) mentioned above. In the latter case, when detailed calculations warrant finding stresses and strains at the cell level, a numerical method, such as the finite element method is employed. In those instances, a large number of elements are required to perform the discrete cell level calculations. It is therefore desirable to develop a continuum level characterization for the honeycomb, as has been detailed in Ref With regard to the development of a continuum model, one issue that has been overlooked is the scaling of honeycomb properties with respect to cell size. That is, one requires identifying certain geometrically based repeating units of the honeycomb (representative unit cell RUC) and establishing the independence (or lack thereof) of honeycomb properties with respect to the number of such RUC s. By definition, RUC properties should be scalable for a large number of cells. This was the focus of work reported in Ref. 1, where preliminary results that focused on the size effects in the out of plane compressive crushing of circular cell polycarbonate (PC) honeycomb were presented. The current paper expands upon this study. The results from a new experimental program with several improvements over the original will be presented and discussed. The out of plane response as a function of * Graduate Research Assistant, Aerospace Engineering, University of Michigan, Ann Arbor, MI Student Member, AIAA. Professor of Aerospace Engineering, University of Michigan, Ann Arbor, MI Associate Fellow, AIAA. 1 Copyright 2004 by Erik C. Mellquist and Anthony M. Waas. Published by the, Inc., with permission.
2 specimen size and shape will be discussed. In addition, a numerical model based on the finite element method and aimed at predicting sample behavior will be presented. II. Laboratory Tests A. Honeycomb Test Samples Test samples were made of polycarbonate circular cell honeycomb purchased from Plascore, in Zeeland, MI. This is the same material that was studied in Ref The individual cells have a radius of inches and a wall thickness of x 103 inches. The honeycomb sample has an out of plane height of 1.0 inch. The polycarbonate, assumed isotropic, has the following material properties: Young s Modulus, E= ksi, and Poisson s ratio n=0.3. Test samples were carefully prepared individually by hand so that the external walls were free from broken cells and remnants of the cells they were cut away from. Samples were cut into twentyfour different sizes. The size was quantified by the number of cells (N) that the sample contained. All sizes between one cell and fourteen cells (N=114) were studied. The honeycombs were attached directly to the loading frame by setting the ends of the honeycombs in 1/8 th inch of epoxy. The samples were placed under a light load while the epoxy was setting to insure that a strong bond was formed. In the initial work 1, which studied honeycombs ranging in size from 1 cell to 169 cells, pieces of flat aluminum were glued to the top and bottom of each honeycomb surface with epoxy in order to clamp them during the testing. These samples were placed within the loading frame, but were not attached to it. The new setup guarantees that the honeycombs remained rigidly attached to the loading frame during testing. This allows for data to be recorded while the honeycombs are being unloaded. A comparison of the original and updated setup is shown in Figure 1. B. Test Method A screw driven testing machine was used to perform the crush experiments. Uniaxial out of plane compressive quasistatic loads were measured under displacement control conditions with the use of a load cell. The rigid load frame crush platen movement and a LVDT were used to calculate the macroscopic strain * based on the total contraction at any point in time during crushing. Measurements were taken at a sampling rate greater than 2 Hz. Each sample was loaded until it was crushed at least 1/4 of an inch (or a macroscopic strain of 0.33). Figure 2 shows pictures of undeformed and deformed honeycombs containing seven cells (N=7). After the honeycombs were loaded they were immediately unloaded until the load decreased to zero. In several tests the honeycombs were loaded and unloaded multiple times. C. Material Behavior The behavior of all the samples was characterized by an initial period of stiff linear response followed by the achievement of a maximum stress (S max ). During this period, the load rose very quickly until a macroscopic strain of about 0.02 was reached. At this point the load reached its maximum value. When this occurred, there was no noticeable deformation. Immediately after the maximum load was reached, a welldefined localized buckle formed around the circumference of the honeycombs. The buckle pattern was located a short distance (approximately 0.2 inches from the top edge of the specimens, in the crush direction). At this point, the load dropped very quickly. After this, the single buckle zone began expanding along the crushing axis of the honeycombs, and a sizable region of crush (a crush zone) at a constant state of stress (plateau stress (S plateau )) was observed. After a plateau stress had been reached the honeycombs were unloaded until the load reached zero. During the unloading period, the crush zones lengthened slightly. After loading and unloading were complete the honeycombs remained significantly shorter than they were originally, indicating that energy had been absorbed. A typical response diagram in macroscopic stressmacroscopic strain space is as indicated in Figure 3 (S max and S plateau are also shown) for a honeycomb sample with N=7. III. Experimental Results A. Scaling Results * Macroscopic strain is defined as crush displacement divided by the original length of the specimen. The resulting macroscopic stressstrain curve is similar to the P_ curve in a stability problem. 2
3 A total of approximately 150 specimens were tested (from both the first and second study). The results were analyzed by examining the macroscopic stressstain response of each honeycomb sample tested. In order to calculate stress, the loading area of a honeycomb sample was considered to be the area contained within the outer edges of the sample. We focused our study on two major properties of every test, S max and S plateau. It was previously reported 1 that S max was highest for N=7. The results of this set of tests (with the load introduction boundaries attached to the loading frame) show that there is not enough evidence to support a claim that a sample with seven cells has a higher S max than a sample of another number of cells. It was seen that S max can vary, sometimes greatly, from one test to another for similar samples. Figure 4 shows the average S max and S plateau for all the samples tested (N = 1 14). Observing the results in Figure 4, we notice that the S plateau was much more consistent than S max. From this we deduced that S max is highly sensitive to imperfections in the samples. Since the maximum load corresponds to a highly unstable buckling type event, it makes sense that S max (directly correlated to the maximum buckling load) would be imperfection sensitive and different in every test. B. Stability Analyses After it was determined that imperfections in the honeycomb samples had a large effect on the results, samples were studied to see if there was a correlation between a sample s shape and the imperfection sensitivity of that sample. Table 1 contains sketches of sample shapes, and number of lines of symmetry. Symmetry is based on the geometric symmetry of the figures shown. By comparing Table 1 to the scaling results from Figure 4 it can be seen that the more lines of symmetry a sample contains, the more likely it is to have a smaller error range. A more symmetric sample is less sensitive to imperfections, which causes the sample to perform similarly every time it is loaded. Another way to characterize the spatial distribution of material in a cellular structure like honeycomb is to use the notion of the fabric tensor 4. However, for such a characterization, one needs to have a sufficiently large number of cells within the crosssection to construct the fabric tensor. For samples with N=7 or greater and assuming radial periodicity every 60, the fabric tensor for the circular cell honeycombs that have been studied is shown in Figure 5. C. Energy Absorption Since honeycomb structures are often used in an energy absorption role, the scaling of energy absorption with honeycomb size was studied. Using the loadingunloading data obtained during experiments, the energy absorbed per unit of permanent deformation was calculated. Energy absorbed was calculated as the area under the loaddisplacement curve. The permanent deformation was considered to be the length that a honeycomb had shortened once the load had been reduced to zero after crushing. The results are presented in Figure 6. Figure 6 shows that there does not appear to be a scaling effect of energy absorption. This is because it depends mostly on plateau stress, and this stress is found to be independent (within statistical significance) of the number of cells, N. Since the plateau stress is independent of cell size, different honeycomb sizes and configurations do not have a great effect on this quantity. IV. Finite Element Analysis In order to check the accuracy of the laboratory tests, a finite element model of the honeycomb was developed using the commercial software packages SDRCIDEAS and Abaqus. Thin shell, eightnoded elements were used to create a sevencell honeycomb model. This model was used to determine the proper material and simulation properties that would be used in future FEA simulations. After it was determined that these model and simulation properties were satisfactory, models containing 1, 3, 4, 5, and 9 cells were created and analyzed. The analyses were carried out in Abaqus using nonlinear geometry and the Riks method option. The Riks method recalculates the model stiffness matrix at every specified time step allowing all equilibrium solutions (stable and unstable) to be captured. The models were analyzed using boundary displacement loading as was done in the experiments. A picture of the original sevencell model before and after loading is shown in Figure 7. The picture shows that deformation predicted in the FEA simulations is similar to what was seen in the experiments. As stated earlier, with buckling problems, initial geometric imperfections have a strong effect on the maximum buckling load. It is also known that nonlinearity in the material response curve also has an effect on the maximum buckling load. These two properties were studied and altered accordingly until the resulting FEA response closely matched the experimental response. Geometric imperfection was introduced to the model by performing an eigenmode analyses in Abaqus to determine the lowest 3 axial buckling modes. The mode corresponding to the smallest eigenvalue was used as an 3
4 initial imperfection shape and the perfect shell mesh was perturbed by a predetermined magnitude of this lowest eigenmode shape. It was determined that an imperfection magnitude of 0.2% of the shell thickness produced the best agreement with the experimental results. Material nonlinearity was introduced to the model using J2 incremental theory of plasticity 3. To determine the material properties of polycarbonate, several tensile loading tests were performed on single circular polycarbonate cells. The results are shown in Figure 8 along with polycarbonate properties that were presented in Ref. 2. From these results, an acceptable range of material stiffness was determined. Using J2 incremental theory of plasticity the material response was modeled using a piecewise linear uniaxial stressstrain curve which is also shown in Figure 8. Initially, the slopes of the elastic and plastic parts of the curve were held as variables. Many test simulations were done to determine the slopes that produced the closest agreement with experiment. Ultimately it was found that slopes of 273 Ksi for the elastic part of the curve and 53 Ksi for the plastic part of the curve generated the best similarity to the experimental results. A graph comparing the FEA results to three sets of experimental results is shown in Figure 9. The FE results predict a maximum load of approximately 75 lbs., which is in the range of the experimentally measured values. The simulation was unable to properly predict the plateau load that was seen during experiments. An investigation into reasons for this discrepancy is ongoing. After the finite element model and the method used to analyze it were verified for the seven cell honeycomb, the model was expanded for other sizes of honeycomb. Figure 10 shows the scaling results for S max for both experiments and finite element simulations. The graph shows good correlation between the results. V. Conclusion The effect of out of plane crushing on circular cell polycarbonate honeycombs has been studied experimentally and numerically. The results show that number of cells does not have an effect on the compressive strength (per unit area) of the honeycomb, but that the way that the cells are arranged does have an effect on the response. Samples that were determined to be more stable are less sensitive to imperfection and produce results that are less varied. Finite element analysis was used to simulate the behavior of the honeycombs during crushing. The FEA results are in good agreement with the experimental results for the six different honeycomb sizes that were studied. References 1 E. C. Mellquist and A. M. Waas, Size Effects In the Compressive Crushing Of Honeycombs, AIAA SDM J. Chung and A. M. Waas, Inplane biaxial crush response of polycarbonate honeycombs, J. Engrg. Mech., ASCE, Vol. 127, No. 2, pp. 180, J. Chung and A. M. Waas, Compressive response and failure of circular cell polycarbonate honeycombs under inplane uniaxial stresses, J. Eng. Mat. Tech., Vol. 121, No. 4, pp. 494, M. Oda, J. Konishi and S. NematNasser, Some experimentally based fundamental results on the mechanical behavior of granular materials,geotechnique., Vol. 30, pp. 479,
5 Loading Platen Honeycomb (a) (b) Figure 1. Original and New Test Setup. In the original setup (a), the honeycomb was attached to flat plates, which were not attached to the loading platen. In the new setup (b), the honeycomb was set in (1/8 th in deep) loading blocks, which were rigidly attached to the loading platen. 1.0 in. Figure 2. Undeformed and Deformed Honeycombs (N=7). 5
6 S max S plateau S (psi) Figure 3. A typical response diagram for N=7. e 6
7 Stress (psi) Max Stress Plateau Stress Number of Cells Figure 4. Scaling Of Honeycomb Properties. Both S max and S plateau are shown. The error bars indicate the range of results for a given number of cells. The error for the plateau stress is much lower than for maximum stress indicating that S max is more sensitive to imperfections in the sample. 7
8 Number of Cells Cell Shape Lines of Symmetry 1 Infinite (+2 flip symmetry lines)
9 (+2 flip symmetric lines) (+2 flip symmetric lines) 14 1 Table 1. Sample Shapes And Symmetry. Solid lines drawn through the pictures indicate lines of geometric symmetry. Dashed lines indicate lines of flip symmetry. These lines go through the geometric centroid of the sample and leave equal amounts of area on both sides of the line. 9
10 0.02 inches 0.01 inches Figure 5. The Fabric Tensor For a Honeycomb Sample With an Infinite Number Of Cells. The mean intercept length is shown based on direction. The inset picture shows the direction indicated as 0. 10
11 Energy Absorbed Per Unit Volume Of Crushed Material (inlbs/in ) Number of Cells Figure 6. Scaling of Energy Absorption. The graph shows that the energy that a honeycomb absorbs during crushing is not affected by the number of cells. 11
12 Figure 7. Undeformed And Deformed Finite Element Models. The slight eigenmode imperfection can be seen in the undeformed model. The deformed model shows the same buckle pattern that was seen in the experiments. From Ref. 2 Figure 8. Material Properties Of Polycarbonate. Based on experimental data and the curve from Ref. 2 an upper and lower bound for material properties were established. By working within these boundaries, a suitable material properties curve was found for the finite element analysis. 12
13 Figure 9. Comparison Of Finite Element And Experimental Results. The FEA results show good prediction of the maximum load, but are unable to capture the plateau load results. 13
14 Stress (psi) Experimental Max Stress FEA Max Stress Number of Cells Figure 10. Maximum Load Scaling For Finite Element Results. The FEA results correlate well with the experimental results. 14
Machine Direction Strength Theory of Corrugated Fiberboard
Thomas J. Urbanik 1 Machine Direction Strength Theory of Corrugated Fiberboard REFERENCE: Urbanik.T.J., Machine Direction Strength Theory of Corrugated Fiberboard, Journal of Composites Technology & Research,
More informationTesting and Analysis
Testing and Analysis Testing Elastomers for Hyperelastic Material Models in Finite Element Analysis 2.6 2.4 2.2 2.0 1.8 1.6 1.4 Biaxial Extension Simple Tension Figure 1, A Typical Final Data Set for Input
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationLecture #10: Anisotropic plasticity Crashworthiness Basics of shell elements
Lecture #10: 1510735: Dynamic behavior of materials and structures Anisotropic plasticity Crashworthiness Basics of shell elements by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering,
More informationLateral Crushing of Square and Rectangular Metallic Tubes under Different QuasiStatic Conditions
Vol:, No:1, 2 Lateral Crushing of Square and Rectangular Metallic Tubes under Different QuasiStatic Conditions Sajjad Dehghanpour, Ali Yousefi International Science Index, Mechanical and Mechatronics
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationBuckling, Postbuckling, and Collapse Analysis with Abaqus. Abaqus 2017
Buckling, Postbuckling, and Collapse Analysis with Abaqus Abaqus 2017 About this Course Course objectives Upon completion of this course you will be able to: Perform linear eigenvalue buckling analysis
More informationNonlinear Buckling Prediction in ANSYS. August 2009
Nonlinear Buckling Prediction in ANSYS August 2009 Buckling Overview Prediction of buckling of engineering structures is a challenging problem for several reasons: A real structure contains imperfections
More informationSolid Mechanics Homework Answers
Name: Date: Solid Mechanics Homework nswers Please show all of your work, including which equations you are using, and circle your final answer. Be sure to include the units in your answers. 1. The yield
More informationTask 1  Material Testing of Bionax Pipe and Joints
Task 1  Material Testing of Bionax Pipe and Joints Submitted to: Jeff Phillips Western Regional Engineer IPEX Management, Inc. 20460 Duncan Way Langley, BC, Canada V3A 7A3 Ph: 6045348631 Fax: 6045347616
More informationGLOBAL AND LOCAL LINEAR BUCKLING BEHAVIOR OF A CHIRAL CELLULAR STRUCTURE
GLOBAL AND LOCAL LINEAR BUCKLING BEHAVIOR OF A CHIRAL CELLULAR STRUCTURE Alessandro Spadoni, Massimo Ruzzene School of Aerospace Engineering Georgia Institute of Technology Atlanta, GA 30332 Fabrizio Scarpa
More informationDate Submitted: 1/8/13 Section #4: T Instructor: Morgan DeLuca. Abstract
Lab Report #2: Poisson s Ratio Name: Sarah Brown Date Submitted: 1/8/13 Section #4: T 1012 Instructor: Morgan DeLuca Group Members: 1. Maura Chmielowiec 2. Travis Newberry 3. Thomas Cannon Title: Poisson
More informationUniaxial Loading: Design for Strength, Stiffness, and Stress Concentrations
Uniaxial Loading: Design for Strength, Stiffness, and Stress Concentrations Lisa Hatcher This overview of design concerning uniaxial loading is meant to supplement theoretical information presented in
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationThe design of a formula student front impact attenuator
The design of a formula student front impact attenuator J.M.J. Schormans MT 10.06 Supervisors: dr. ir. Varvara Kouznetsova Eindhoven University of Technology Department of Mechanical Engineering Computational
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationChapter 5. Vibration Analysis. Workbench  Mechanical Introduction ANSYS, Inc. Proprietary 2009 ANSYS, Inc. All rights reserved.
Workbench  Mechanical Introduction 12.0 Chapter 5 Vibration Analysis 51 Chapter Overview In this chapter, performing free vibration analyses in Simulation will be covered. In Simulation, performing a
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationIntroduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams.
Outline of Continuous Systems. Introduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams. Vibrations of Flexible Strings. Torsional Vibration of Rods. BernoulliEuler Beams.
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationEXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS
EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown,
More informationBehavior of Tubular Hat Structure Under Three Point Bending
International Journal of Transportation Engineering and Technology 2016; 2(51): 1824 http://www.sciencepublishinggroup.com j/ijtet doi: 10.11648/j.ijtet.s.2016020501.14 Behavior of Tubular Hat Structure
More informationMINIMUM WEIGHT STRUCTURAL SANDWICH
U.S. DEPARTMENT OF AGRICULTURE FOREST SERVICE FOREST PRODUCTS LABORATORY MADISON, WIS. In Cooperation with the University of Wisconsin U.S.D.A. FOREST SERVICE RESEARCH NOTE Revised NOVEMBER 1970 MINIMUM
More informationNonlinear Analysis Of An EPDM Hydraulic Accumulator Bladder. Richard Kennison, RaceTec
Nonlinear Analysis Of An EPDM Hydraulic Accumulator Bladder Richard Kennison, RaceTec Agenda RaceTec Overview Accumulator Experimental Testing Material Testing Numerical Analysis: 1. Linear Buckling
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationDynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models
Dynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models I. Rhee, K.J. Willam, B.P. Shing, University of Colorado at Boulder ABSTRACT: This paper examines the global
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More informationTINIUS OLSEN Testing Machine Co., Inc.
Interpretation of StressStrain Curves and Mechanical Properties of Materials Tinius Olsen has prepared this general introduction to the interpretation of stressstrain curves for the benefit of those
More informationACET 406 MidTerm Exam B
ACET 406 MidTerm Exam B SUBJECT: ACET 406, INSTRUCTOR: Dr Antonis Michael, DATE: 24/11/09 INSTRUCTIONS You are required to answer all of the following questions within the specified time (90 minutes).you
More informationAdaptive Analysis of Bifurcation Points of Shell Structures
First published in: Adaptive Analysis of Bifurcation Points of Shell Structures E. Ewert and K. Schweizerhof Institut für Mechanik, Universität Karlsruhe (TH), Kaiserstraße 12, D76131 Karlsruhe, Germany
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationThe Design of Polyurethane Parts: Using Closed Solutions and Finite Element Analysis to Obtain Optimal Results
The Design of Polyurethane Parts: Using Closed Solutions and Finite Element Analysis to Obtain Optimal Results By: Richard Palinkas George Nybakken Ian Laskowitz Chemtura Corporation Overview How does
More informationTolerance Ring Improvement for Reducing Metal Scratch
International Journal of Scientific and Research Publications, Volume 2, Issue 11, November 2012 1 Tolerance Ring Improvement for Reducing Metal Scratch Pattaraweerin Woraratsoontorn*, Pitikhate Sooraksa**
More information1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine Spring 2004 LABORATORY ASSIGNMENT NUMBER 6
1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine MIT Spring 2004 LABORATORY ASSIGNMENT NUMBER 6 COMPRESSION TESTING AND ANISOTROPY OF WOOD Purpose: Reading: During this laboratory
More informationUnified Quiz M4 May 7, 2008 M  PORTION
9:0010: 00 (last four digits) 32141 Unified Quiz M4 May 7, 2008 M  PORTION Put the last four digits of your MIT ID # on each page of the exam. Read all questions carefully. Do all work on that question
More informationGerald Allen Cohen, 83, passed away Oct. 1, 2014, at his home in Laguna Beach.
Dr Gerald Allen Cohen (19312014) Ringstiffened shallow conical shell designed with the use of FASOR for NASA s Viking project in the 1970s. (from NASA TN D7853, 1975, by Walter L. Heard, Jr., Melvin
More informationVibration Transmission in Complex Vehicle Structures
Vibration Transmission in Complex Vehicle Structures Christophe Pierre Professor Matthew P. Castanier Assistant Research Scientist YungChang Tan Dongying Jiang Graduate Student Research Assistants Vibrations
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationDesign of a Cheap Thermal Switch. ENGR 0135 Due: 10/9/15 Professor QingMing Wang Madison Milligan, Josh Haupt, Caroline Collopy
Design of a Cheap Thermal Switch ENGR 0135 Due: 10/9/15 Professor QingMing Wang Madison Milligan, Josh Haupt, Caroline Collopy ABSTRACT The purpose of this design project is to come up with a way to develop
More informationElasticity: Term Paper. Danielle Harper. University of Central Florida
Elasticity: Term Paper Danielle Harper University of Central Florida I. Abstract This research was conducted in order to experimentally test certain components of the theory of elasticity. The theory was
More informationOn MooneyRivlin Constants for Elastomers
th International LSDYNA Users Conference Constitutive Modeling() On Mooneyivlin Constants for Elastomers The Mooneyivlin constitutive equation for rubber is W C I C I 3 3 William W. Feng John O. Hallquist
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationKnockdown Factors for Buckling of Cylindrical and Spherical Shells Subject to Reduced Biaxial Membrane Stress
Knockdown Factors for Buckling of Cylindrical and Spherical Shells Subject to Reduced Biaxial Membrane Stress The Harvard community has made this article openly available. Please share how this access
More informationNumerical modelling of induced tensile stresses in rock in response to impact loading
Numerical modelling of induced tensile stresses in rock in response to impact loading M.T. Mnisi, D.P. Roberts and J.S. Kuijpers Council for Scientific and Industrial Research (CSIR): Natural Resources
More information8/1/2009. CAE 7962 Presentation
CAE 7962 Presentation Gavin Patey Dameion Moores Aaron Henstridge Ashley Burke Brendan Harvey Fabio Faragalli Introduction Choosing mesh properties Explanation of the types of studies available and the
More informationBME 207 Introduction to Biomechanics Spring 2017
April 7, 2017 UNIVERSITY OF RHODE ISAND Department of Electrical, Computer and Biomedical Engineering BE 207 Introduction to Biomechanics Spring 2017 Homework 7 Problem 14.3 in the textbook. In addition
More informationLecture 7, Foams, 3.054
Lecture 7, Foams, 3.054 Opencell foams StressStrain curve: deformation and failure mechanisms Compression  3 regimes  linear elastic  bending  stress plateau  cell collapse by buckling yielding
More informationCOUPLED USE OF FEA AND EMA FOR THE INVESTIGATION OF DYNAMIC BEHAVIOUR OF AN INJECTION PUMP
COUPLED USE OF FEA AND EMA FOR THE INVESTIGATION OF DYNAMIC BEHAVIOUR OF AN INJECTION PUMP Yasar Deger Wolfram Lienau Peter Sandford Sulzer Markets & Sulzer Pumps Ltd Sulzer Pumps (UK) Ltd Technology Ltd
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationNonlinear Analysis of Reinforced Concrete Shells Subjected to Impact Loads
Transactions of the 7 th International Conference on Structural Mechanics in Reactor Technology (SMiRT 7) Prague, Czech Republic, August 7, 00 Paper # J0 Nonlinear Analysis of Reinforced Concrete Shells
More informationSUITABILITY OF USING CALIFORNIA BEARING RATIO TEST TO PREDICT RESILIENT MODULUS
SUITABILITY OF USING CALIFORNIA BEARING RATIO TEST TO PREDICT RESILIENT MODULUS By: Beena Sukumaran, Associate Professor, Civil & Environmental Engineering Rowan University 201 Mullica Hill Road, Glassboro,
More informationFINITE ELEMENT MODELING OF WOOD DIAPHRAGMS
FINITE ELEMENT MODELING OF WOOD DIAPHRAGMS By Robert H. Falk 1 and Rafii Y. Itani, 2 Member, ASCE ABSTRACT: This report describes a twodimensional finite element model for analyzing vertical and horizontal
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationMATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?
MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition
More informationTHE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE
Journal of Applied Mathematics and Computational Mechanics 013, 1(4), 131 THE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE Jolanta Błaszczuk
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationEffect of Strain Hardening on Unloading of a Deformable Sphere Loaded against a Rigid Flat A Finite Element Study
Effect of Strain Hardening on Unloading of a Deformable Sphere Loaded against a Rigid Flat A Finite Element Study Biplab Chatterjee, Prasanta Sahoo 1 Department of Mechanical Engineering, Jadavpur University
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationSHELL STRUCTURES. THEORY AND APPLICATIONS
The 5th Conference SHELL STRUCTURES. THEORY AND APPLICATIONS Janowice * 1518 October MODERATE ROTATION THEORY FEM ANALYSIS OF LAMINATED ANISOTROPIC COMPOSITE PLATES AND SHELLS I. Kreja 1 ) and R. Schmidt
More informationRESEARCH PROJECT NO. 26
RESEARCH PROJECT NO. 26 DETERMINATION OF POISSON'S RATIO IN AD1 TESTING BY UNIVERSITY OF MICHIGAN REPORT PREPARED BY BELA V. KOVACS and JOHN R. KEOUGH \ MEMBER / / DUCTILE IRON \ SOCIETY Issued by the
More informationDEVELOPMENT OF DROP WEIGHT IMPACT TEST MACHINE
CHAPTER8 DEVELOPMENT OF DROP WEIGHT IMPACT TEST MACHINE 8.1 Introduction The behavior of materials is different when they are subjected to dynamic loading [9]. The testing of materials under dynamic conditions
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationIMECE CRACK TUNNELING: EFFECT OF STRESS CONSTRAINT
Proceedings of IMECE04 2004 ASME International Mechanical Engineering Congress November 1320, 2004, Anaheim, California USA IMECE200460700 CRACK TUNNELING: EFFECT OF STRESS CONSTRAINT Jianzheng Zuo Department
More informationtwo structural analysis (statics & mechanics) APPLIED ACHITECTURAL STRUCTURES: DR. ANNE NICHOLS SPRING 2017 lecture STRUCTURAL ANALYSIS AND SYSTEMS
APPLIED ACHITECTURAL STRUCTURES: STRUCTURAL ANALYSIS AND SYSTEMS DR. ANNE NICHOLS SPRING 2017 lecture two structural analysis (statics & mechanics) Analysis 1 Structural Requirements strength serviceability
More information#SEU16. FEA in Solid Edge and FEMAP Mark Sherman
FEA in Solid Edge and FEMAP Mark Sherman Realize innovation. FEMAP Continuous development with the same core team! Since 1985 there have been more than 35 releases of FEMAP with only one major architecture
More informationOptimum Fiber Distribution in Singlewall Corrugated Fiberboard
United States Department of Agriculture Forest Service Forest Products Laboratory Research Paper FPL 348 1979 Optimum Fiber Distribution in Singlewall Corrugated Fiberboard Abstract Determining optimum
More informationFASTENER SPACING STUDY OF COLDFORMED STEEL WALL STUDS USING FINITE STRIP AND FINITE ELEMENT METHODS
FASTENER SPACING STUDY OF COLDFORMED STEEL WALL STUDS USING FINITE STRIP AND FINITE ELEMENT METHODS RESEARCH REPORT Brian Post Dept. of Civil Engineering Johns Hopins University December 202 .0 INTRODUCTION
More informationMECHANICAL PROPERTIES OF SOLIDS
Chapter Nine MECHANICAL PROPERTIES OF SOLIDS MCQ I 9.1 Modulus of rigidity of ideal liquids is (a) infinity. (b) zero. (c) unity. (d) some finite small nonzero constant value. 9. The maximum load a wire
More informationStress Analysis on Bulkhead Model for BWB Heavy Lifter Passenger Aircraft
The International Journal Of Engineering And Science (IJES) Volume 3 Issue 01 Pages 3843 014 ISSN (e): 319 1813 ISSN (p): 319 1805 Stress Analysis on Bulkhead Model for BWB Heavy Lifter Passenger Aircraft
More informationMAXIMUM ENTROPYBASED UNCERTAINTY MODELING AT THE FINITE ELEMENT LEVEL. Pengchao Song and Marc P. Mignolet
MAXIMUM ENTROPYBASED UNCERTAINTY MODELING AT THE FINITE ELEMENT LEVEL Pengchao Song and Marc P. Mignolet SEMTE, Faculties of Mechanical and Aerospace Engineering, Arizona State University, 51 E. Tyler
More informationCivil Engineering Design (1) Design of Reinforced Concrete Columns 2006/7
Civil Engineering Design (1) Design of Reinforced Concrete Columns 2006/7 Dr. Colin Caprani, Chartered Engineer 1 Contents 1. Introduction... 3 1.1 Background... 3 1.2 Failure Modes... 5 1.3 Design Aspects...
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationThe Local Web Buckling Strength of Coped Steel IBeam. ABSTRACT : When a beam flange is coped to allow clearance at the
The Local Web Buckling Strength of Coped Steel IBeam Michael C. H. Yam 1 Member, ASCE Angus C. C. Lam Associate Member, ASCE, V. P. IU and J. J. R. Cheng 3 Members, ASCE ABSTRACT : When a beam flange
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationLab Exercise #3: Torsion
Lab Exercise #3: Prelab assignment: Yes No Goals: 1. To evaluate the equations of angular displacement, shear stress, and shear strain for a shaft undergoing torsional stress. Principles: testing of round
More informationModified Symmetry Cell Approach for Simulation of Surface Enhancement Over Large Scale Structures
Modified Symmetry Cell Approach for Simulation of Surface Enhancement Over Large Scale Structures T. Spradlin 1, R. Grandhi 2, and K. Langer 3 1 Doctoral Candidate, Wright State University, USA 2 Distinguished
More informationArberi Ferraj. Wentworth Institute of Technology. Design of Machine Elements MECH 420
P a g e 1 Arberi Ferraj Wentworth Institute of Technology Design of Machine Elements MECH 420 P a g e 2 1. Executive Summary A scissor car jack was designed and must be reverseengineered in order to discover
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationIntensity (a.u.) Intensity (a.u.) Raman Shift (cm 1 ) Oxygen plasma. 6 cm. 9 cm. 1mm. Singlelayer graphene sheet. 10mm. 14 cm
Intensity (a.u.) Intensity (a.u.) a Oxygen plasma b 6 cm 1mm 10mm Singlelayer graphene sheet 14 cm 9 cm Flipped Si/SiO 2 Patterned chip Plasmacleaned glass slides c d After 1 sec normal Oxygen plasma
More informationRESILIENT INFRASTRUCTURE June 1 4, 2016
RESILIENT INFRASTRUCTURE June 1 4, 2016 DAMAGE DETECTION OF UHPFRC PLATES USING RANDOM DECREMENT TECHNIQUE Azita Pourrastegar MASc Student, Ryerson University, azita2.pourrastegar@ryerson.ca, Canada Hesham
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationMechanical Design in Optical Engineering
OPTI Buckling Buckling and Stability: As we learned in the previous lectures, structures may fail in a variety of ways, depending on the materials, load and support conditions. We had two primary concerns:
More informationMECH 344/X Machine Element Design
1 MECH 344/X Machine Element Design Time: M 14:4517:30 Lecture 2 Contents of today's lecture Introduction to Static Stresses Axial, Shear and Torsional Loading Bending in Straight and Curved Beams Transverse
More informationInvestigation of the Shear Thickening Fluid Dynamic Properties and its Influence on the Impact Resistance of Multilayered Fabric Composite Barrier
11 th International LSDYNA Users Conference Blast / Impact (1) Investigation of the Shear Thickening Fluid Dynamic Properties and its Influence on the Impact Resistance of Multilayered Fabric Composite
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationFinite Element Solutions for Geotechnical Engineering
Release Notes Release Date: July, 2015 Product Ver.: GTSNX 2015 (v2.1) Integrated Solver Optimized for the next generation 64bit platform Finite Element Solutions for Geotechnical Engineering Enhancements
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationFinite Element Analysis of Buckling of Corrugated Fiberboard
Send Orders for Reprints to reprints@benthamscience.ae The Open Mechanical Engineering Journal, 2014, 8, 257263 257 Finite Element Analysis of Buckling of Corrugated Fiberboard Yali Ma *,1, Zhen Gong
More informationBUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION
2 th International Conference on Composite Materials Copenhagen, 1924 th July 215 BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr.
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More information548 Advances of Computational Mechanics in Australia
Applied Mechanics and Materials Online: 20160725 ISSN: 16627482, Vol. 846, pp 547552 doi:10.4028/www.scientific.net/amm.846.547 2016 Trans Tech Publications, Switzerland Geometric bounds for bucklinginduced
More informationNonlinear analysis in ADINA Structures
Nonlinear analysis in ADINA Structures Theodore Sussman, Ph.D. ADINA R&D, Inc, 2016 1 Topics presented Types of nonlinearities Materially nonlinear only Geometrically nonlinear analysis Deformationdependent
More information